False Nettle, Water Boil Stem With Potassium Carbonate, Peel Fiber

Source: Comparative Plant Fiber Collection
FN-032-08-25-09-BF-400X-PM-4-9 	
{| Class="wikitable" border="1" style="border-collapse:collapse;"
Source 	bast
Accession Number 	8/4/93-AE.142.1.1-29.4.1-4.8/19/93 (O) #802
Title 	False nettle, water boil stem in potassium carbonate, peel fiber
Processing treatment 	boil in water with potassium carbonate
Image Identification information	FN-032-08-25-09-BF-400X-PM-4-9
Image capture 	digital
Date of image capture 	08/25/09
Microscopist 	L. Crawford
Microscope 	Zeiss Axioplan
Mounting agent and RI 	RI: permoint 1.515
Microscopic technique 	Brightfield
Lumen type 	wide lumen diameter relative to fiber diameter
Lumen filling 	irregular lumen filling
Dislocations 	few dislocations
Fiber size 	wide fiber diameter
Surface folds 	surface folds present
Cambium 	cambium apparent
FN-033-08-25-09-DF-400X-PM-4-9 	
{| Class="wikitable" border="1" style="border-collapse:collapse;"
Source 	bast
Accession Number 	8/4/93-AE.142.1.1-29.4.1-4.8/19/93 (O) #802
Title 	False nettle, water boil stem in potassium carbonate, peel fiber
Processing treatment 	boil in water with potassium carbonate
Image Identification information	FN-033-08-25-09-DF-400X-PM-4-9
Image capture 	digital
Date of image capture 	08/25/09
Microscopist 	L. Crawford
Microscope 	Zeiss Axioplan
Mounting agent and RI 	RI: permount 1.515
Microscopic technique 	Darkfield
Lumen type 	wide lumen diameter relative to fiber diameter
Lumen filling 	irregular lumen filling
Dislocations 	few dislocations
Fiber size 	wide fiber diameter
Surface folds 	surface folds present
Cambium 	cambium apparent
FN-034-08-25-09-POL-400X-PM-4-9	
{| Class="wikitable" border="1" style="border-collapse:collapse;"
Source 	bast
Accession Number 	8/4/93-AE.142.1.1-29.4.1-4.8/19/93 (O) #802
Title 	False nettle, water boil stem in potassium carbonate, peel fiber
Processing treatment 	boil in water with potassium carbonate
Image Identification information	FN-034-08-25-09-POL-400X-PM-4-9
Image capture 	digital
Date of image capture 	08/25/09
Microscopist 	L. Crawford
Microscope 	Zeiss Axioplan
Mounting agent and RI 	RI: permount 1.515
Microscopic technique 	Polarized light, fiber at maximum brightness
Lumen type 	wide lumen diameter relative to fiber diameter
Lumen filling 	irregular lumen filling
Dislocations 	few dislocations
Fiber size 	wide fiber diameter
Surface folds 	surface folds present
Cambium 	cambium apparent
FN-035-08-25-09-DIC-400X-PM-4-9	
{| Class="wikitable" border="1" style="border-collapse:collapse;"
Source 	bast
Accession Number 	8/4/93-AE.142.1.1-29.4.1-4.8/19/93 (O) #802
Title 	False nettle, water boil stem in potassium carbonate, peel fiber
Processing treatment 	boil in water with potassium carbonate
Image Identification information	FN-035-08-25-09-DIC-400X-PM-4-9
Image capture 	digital
Date of image capture 	08/25/09
Microscopist 	L. Crawford
Microscope 	Zeiss Axioplan
Mounting agent and RI 	RI: permount 1.515
Microscopic technique 	Differential interference contrast
Lumen type 	wide lumen diameter relative to fiber diameter
Lumen filling 	irregular lumen filling
Dislocations 	few dislocations
Fiber size 	wide fiber diameter
Surface folds 	surface folds present
Cambium 	cambium apparent
FN-036-08-25-09-POL-400X-PM-4-9	
{| Class="wikitable" border="1" style="border-collapse:collapse;"
Source 	bast
Accession Number 	8/4/93-AE.142.1.1-29.4.1-4.8/19/93 (O) #802
Title 	False nettle, water boil stem in potassium carbonate, peel fiber
Processing treatment 	boil in water with potassium carbonate
Image Identification information	FN-036-08-25-09-POL-400X-PM-4-9
Image capture 	digital
Date of image capture 	08/25/09
Microscopist 	L. Crawford
Microscope 	Zeiss Axioplan
Mounting agent and RI 	RI: permount 1.515
Microscopic technique 	Polarized light, fiber at extinction
Lumen type 	wide lumen diameter relative to fiber diameter
Lumen filling 	irregular lumen filling
Dislocations 	few dislocations
Fiber size 	wide fiber diameter
Surface folds 	surface folds present
Cambium 	cambium apparent
FN-037-08-25-09-POL_FOR-400X-PM-4-9	
{| Class="wikitable" border="1" style="border-collapse:collapse;"
Source 	bast
Accession Number 	8/4/93-AE.142.1.1-29.4.1-4.8/19/93 (O) #802
Title 	False nettle, water boil stem in potassium carbonate, peel fiber
Processing treatment 	boil in water with potassium carbonate
Image Identification information	FN-037-08-25-09-POL_FOR-400X-PM-4-9
Image capture 	digital
Date of image capture 	08/25/09
Microscopist 	L. Crawford
Microscope 	Zeiss Axioplan
Mounting agent and RI 	RI: permount 1.515
Microscopic technique 	Polarized light, First Order Red plate, exaggerated brightness
Lumen type 	wide lumen diameter relative to fiber diameter
Lumen filling 	irregular lumen filling
Dislocations 	few dislocations
Fiber size 	wide fiber diameter
Surface folds 	surface folds present
Cambium 	cambium apparent
FN-037.5-03-09-10-POL-FOR-400X-MM-4-9	
{| Class="wikitable" border="1" style="border-collapse:collapse;"
Source 	bast
Accession Number 	7/11/91 AE. 105.22.2-29.4.1-**-4 10/10/91 (G) 402 #1
Title 	False nettle, water boil stem with potassium carbonate, peel
Processing treatment 	boil in water with potassium carbonate
Image Identification information	FN-037.5-03-09-10-POL-FOR-400X-MM-4-9
Image capture 	digital
Date of image capture 	03/09/10
Microscopist 	L. Crawford
Microscope 	Zeiss Axioplan
Mounting agent and RI 	Meltmount RI 1.539
Microscopic technique 	Polarized light, First Order Red Plate, normal contrast
Lumen type 	lumen not apparent
Fiber size 	medium fiber diameter
FN-038-08-26-09-BF-400X-PM-4-9-overall fibers with crystals	
{| Class="wikitable" border="1" style="border-collapse:collapse;"
Source 	bast
Accession Number 	8/4/93-AE.142.1.1-29.4.1-4.8/19/93 (O) #802
Title 	False nettle, water boil stem in potassium carbonate, peel fiber, fiber and associated materials
Processing treatment 	boil in water with potassium carbonate
Image Identification information	FN-038-08-26-09-BF-400X-PM-4-9-overall fibers with crystals
Image capture 	digital
Date of image capture 	08/25/09
Microscopist 	L. Crawford
Microscope 	Zeiss Axioplan
Mounting agent and RI 	RI: permount 1.515
Microscopic technique 	Brightfield
Lumen type 	wide lumen diameter relative to fiber diameter
Lumen filling 	irregular lumen filling
Dislocations 	few dislocations
Fiber size 	medium fiber diameter
Surface folds 	surface folds present
Crystals 	few crystals
Crystal shape 	2 druse
Cambium 	cambium apparent
FN-039-08-26-09-POL-400X-PM-4-9-overall fibers	
{| Class="wikitable" border="1" style="border-collapse:collapse;"
Source 	bast
Accession Number 	8/4/93-AE.142.1.1-29.4.1-4.8/19/93 (O) #802
Title 	False nettle, water boil stem in potassium carbonate, peel fiber, fiber and associated materials
Processing treatment 	boil in water with potassium carbonate
Image Identification information	FN-039-08-26-09-POL-400X-PM-4-9-overall fibers
Image capture 	digital
Date of image capture 	08/25/09
Microscopist 	L. Crawford
Microscope 	Zeiss Axioplan
Mounting agent and RI 	RI: permount 1.515
Microscopic technique 	Polarized light, fiber at maximum brightness
Lumen type 	wide lumen diameter relative to fiber diameter
Lumen filling 	irregular lumen filling
Dislocations 	few dislocations
Fiber size 	wide fiber diameter
Surface folds 	surface folds present
Cambium 	cambium apparent
FN-040-08-26-09-DIC-400X-PM-4-9-overall fibers	
{| Class="wikitable" border="1" style="border-collapse:collapse;"
Source 	bast
Accession Number 	8/4/93-AE.142.1.1-29.4.1-4.8/19/93 (O) #802
Title 	False nettle, water boil stem in potassium carbonate, peel fiber, fiber and associated materials
Processing treatment 	boil in water with potassium carbonate
Image Identification information	FN-040-08-26-09-DIC-400X-PM-4-9-overall fibers
Image capture 	digital
Date of image capture 	08/25/09
Microscopist 	L. Crawford
Microscope 	Zeiss Axioplan
Mounting agent and RI 	RI: permount 1.515
Microscopic technique 	Differential interference contrast
Lumen type 	wide lumen diameter relative to fiber diameter
Lumen filling 	irregular lumen filling
Dislocations 	few dislocations
Fiber size 	wide fiber diameter
Surface folds 	surface folds present
Cambium 	cambium apparent
FN-041-08-26-09-BF-200X-PM-4-9-overall fibers	
{| Class="wikitable" border="1" style="border-collapse:collapse;"
Source 	bast
Accession Number 	8/4/93-AE.142.1.1-29.4.1-4.8/19/93 (O) #802
Title 	False nettle, water boil stem in potassium carbonate, peel fiber, fiber and associated materials
Processing treatment 	boil in water with potassium carbonate
Image Identification information	FN-041-08-26-09-BF-200X-PM-4-9-overall fibers
Image capture 	digital
Date of image capture 	08/25/09
Microscopist 	L. Crawford
Microscope 	Zeiss Axioplan
Mounting agent and RI 	RI: permount 1.515
Microscopic technique 	Brightfield
Lumen type 	wide lumen diameter relative to fiber diameter
Lumen filling 	irregular lumen filling
Dislocations 	few dislocations
Fiber size 	wide fiber diameter
Surface folds 	surface folds present
Cambium 	cambium apparent
FN-042-08-26-09-BF-400X-PM-4-9-overall fibers w crystals in cambium	
{| Class="wikitable" border="1" style="border-collapse:collapse;"
Source 	bast
Accession Number 	8/4/93-AE.142.1.1-29.4.1-4.8/19/93 (O) #802
Title 	False nettle, water boil stem in potassium carbonate, peel fiber, fiber and associated materials
Processing treatment 	boil in water with potassium carbonate
Image Identification information	FN-042-08-26-09-BF-400X-PM-4-9-overall fibers w crystals in cambium
Image capture 	digital
Date of image capture 	08/25/09
Microscopist 	L. Crawford
Microscope 	Zeiss Axioplan
Mounting agent and RI 	RI: permount 1.515
Microscopic technique 	Brightfield
Lumen type 	wide lumen diameter relative to fiber diameter
Lumen filling 	irregular lumen filling
Dislocations 	few dislocations
Fiber size 	wide fiber diameter
Surface folds 	surface folds present
Crystals 	few crystals
Crystal shape 	2 druse
Cambium 	cambium apparent
FN-043-08-26-09-POL-400X-PM-4-9-overall fibers with crystals in cambium	
{| Class="wikitable" border="1" style="border-collapse:collapse;"
Source 	bast
Accession Number 	8/4/93-AE.142.1.1-29.4.1-4.8/19/93 (O) #802
Title 	False nettle, water boil stem in potassium carbonate, peel fiber, fiber and associated materials
Processing treatment 	boil in water with potassium carbonate
Image Identification information	FN-043-08-26-09-POL-400X-PM-4-9-overall fibers with crystals in cambium
Image capture 	digital
Date of image capture 	08/25/09
Microscopist 	L. Crawford
Microscope 	Zeiss Axioplan
Mounting agent and RI 	RI: permount 1.515
Microscopic technique 	Polarized light, fiber at extinction
Lumen type 	wide lumen diameter relative to fiber diameter
Lumen filling 	irregular lumen filling
Dislocations 	few dislocations
Fiber size 	wide fiber diameter
Surface folds 	surface folds present
Crystals 	few crystals
Crystal shape 	2 druse
Cambium 	cambium apparent
FN-044-08-26-09-DIC-400X-PM-4-9-overall fibers w crystals in cambium	
{| Class="wikitable" border="1" style="border-collapse:collapse;"
Source 	bast
Accession Number 	8/4/93-AE.142.1.1-29.4.1-4.8/19/93 (O) #802
Title 	False nettle, water boil stem in potassium carbonate, peel fiber, fiber and associated materials
Processing treatment 	boil in water with potassium carbonate
Image Identification information	FN-044-08-26-09-DIC-400X-PM-4-9-overall fibers w crystals in cambium
Image capture 	digital
Date of image capture 	08/25/09
Microscopist 	L. Crawford
Microscope 	Zeiss Axioplan
Mounting agent and RI 	RI: permount 1.515
Microscopic technique 	Differential interference contrast
Lumen type 	wide lumen diameter relative to fiber diameter
Lumen filling 	irregular lumen filling
Dislocations 	few dislocations
Fiber size 	wide fiber diameter
Surface folds 	surface folds present
Crystals 	few crystals
Crystal shape 	2 druse
Cambium 	cambium apparent
Category:FRIL
Category: FRIL: False Nettle
Category: FRIL: Plant Fibers